(2) ii. c 2014 Landry Fokoua Djodom All Rights Reserved.

(3) iii. To my family..

(4) iv. Acknowledgments I would like to express my profound gratitude and appreciation to Professor Michael Ortiz for his supervision and guidance throughout my stay at Caltech. I am deeply grateful for his support, his motivation and his patience. He has provided me with a multidisciplinary research experience from which I have learned a lot and his constant encouragement for innovative and challenging ideas has contributed to an exciting PhD work. I would like to specially acknowledge Professor Sergio Conti from the Hausdorff Research Institute of Mathematics, University of Bonn (Germany), for his collaboration throughout this thesis work. I gratefully acknowledge support provided by the Hausdorff Trimester Program “mathematical challenges of materials science and condensed matter physics: From quantum mechanics through statistical mechanics to nonlinear PDEs”, Hausdorff Research Institute for Mathematics (HIM), University of Bonn, Germany. I also gratefully acknowledge the support of the Department of Energy National Nuclear Security Administration through Caltech’s ASC/PSAAP Center for the Predictive Modeling and Simulation of High Energy Density Dynamic Response of Materials. I am particularly thankful to Professor Ravichandran, Professor Bhattacharya and Professor Weinberg for serving on my thesis committee. I would like to thank Professor Andrade and Professor Kochmann for serving on my candidacy exam and for their useful suggestions and comments. I am grateful to Professor Ravichandran for providing insights about my work, for supporting me throughout my stay at GALCIT, and for being a good resource for career aspirations. I thank Professor Weinberg for her feedback, help and useful discussions on my research. During summer 2011, I had the opportunity to spend ten weeks at the Lawrence Livermore.

(5) v National Laboratory. Very warms thanks are addressed to Sylvie Aubry, Tom Arsenlis and Jaime Marian for welcoming me to the lab and exposing me to the exciting field of dislocation dynamics and computational material science. I owe special gratitude to Lydia who has always been available for me, I deeply appreciate her attention and her care which have made my life enjoyable in the office. She has been and will remain a life mentor to me. Special thanks also go to Marta for her availability and help with computer issues. I would also like to acknowledge Cheryl Gause, Dimity Nelson, and Christine Ramirez who have facilitated my insertion into the GALCIT community. I thank the members of my lab group with whom I have had several instructive discussions: Jonathan, Panos, Stephanie, Anie, Gwen, Brandon, Sarah, Jeff, Cindy. My life at Caltech and in the Los Angeles area wouldn’t have been pleasant without the presence of my friends. I owe a sincere acknowledgement to Stephanie, Adam, Ignacio, Jen, Sid, Jomela, Xin, Philipp, Jocelyn, Adrian, Juan, Vicki, Andy, Kristen, Ryan, Cheikh, Gloria, Eleni. I would like to specially acknowledge Terry with whom I have shared many exciting adventures at Caltech and who will remain a close friend. I am deeply grateful to Namiko who has provided me with her presence and attention, and whose friendship will remain precious. I am also thankful to my friends from Santa Barbara, especially Maxime and Kai. Special thanks also to Professor Frédéric Gibou for his support and encouragement since my research internship at the University of California, Santa Barbara. I would like to express my very deep gratitude to Alan and his family who have welcomed me in their lives and I cherish the time that I have spent with them in Pasadena. I am profoundly indebted to Cabral and Ange-Thérèse who I have known during my undergraduate studies in France, and even before, and with whom I have shared a deep friendship over several years. Their continued presence and support have always been invaluable. I thank the Caltech Graduate Student Council which has provided me with the unique opportunity to contribute to the campus life. I am thankful to all the students I collaborated with and I particularly thank Felicia Hunt who has strongly contributed to the success of our events. Finally, but not least, I profoundly thank my family who has always been on my side, and to.

(6) vi whom I simply owe everything..

(7) vii. Abstract This work is concerned with the derivation of optimal scaling laws, in the sense of matching lower and upper bounds on the energy, for a solid undergoing ductile fracture. The specific problem considered concerns a material sample in the form of an infinite slab of finite thickness subjected to prescribed opening displacements on its two surfaces. The solid is assumed to obey deformationtheory of plasticity and, in order to further simplify the analysis, we assume isotropic rigid-plastic deformations with zero plastic spin. When hardening exponents are given values consistent with observation, the energy is found to exhibit sublinear growth. We regularize the energy through the addition of nonlocal energy terms of the strain-gradient plasticity type. This nonlocal regularization has the effect of introducing an intrinsic length scale into the energy. We also put forth a physical argument that identifies the intrinsic length and suggests a linear growth of the nonlocal energy. Under these assumptions, ductile fracture emerges as the net result of two competing effects: whereas the sublinear growth of the local energy promotes localization of deformation to failure planes, the nonlocal regularization stabilizes this process, thus resulting in an orderly progression towards failure and a well-defined specific fracture energy. The optimal scaling laws derived here show that ductile fracture results from localization of deformations to void sheets, and that it requires a well-defined energy per unit fracture area. In particular, fractal modes of fracture are ruled out under the assumptions of the analysis. The optimal scaling laws additionally show that ductile fracture is cohesive in nature, i.e., it obeys a well-defined relation between tractions and opening displacements. Finally, the scaling laws supply a link between micromechanical properties and macroscopic fracture properties. In particular, they reveal the relative roles that surface energy and microplasticity play as contributors to the specific fracture energy of the material. Next, we present.

(8) viii an experimental assessment of the optimal scaling laws. We show that when the specific fracture energy is renormalized in a manner suggested by the optimal scaling laws, the data falls within the bounds predicted by the analysis and, moreover, they ostensibly collapse—with allowances made for experimental scatter—on a master curve dependent on the hardening exponent, but otherwise material independent..

(9) ix. Contents. Acknowledgments. iv. Abstract. vii. Contents. ix. List of Figures. xi. List of Tables. xiii. 1 Introduction 1.1. 1. General overview . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 1. 1.1.1. Experimental observations . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 1. 1.1.2. J -integral testing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 3. 1.1.3. Impact testing . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 4. 1.1.4. Surface energies . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 5. 1.2. Previous work on ductile fracture . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 7. 1.3. Motivation. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 8. 1.4. Outline of the thesis . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 10. 1.5. Mathematical Preliminaries . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 11. 2 From Necking Instability to Strain Gradient Plasticity 2.1. 15. A localization construction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 15. 2.1.1. 16. Uniaxial tension test . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . ..

(10) x. 2.2. 2.1.2. Necking construction . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 19. 2.1.3. Some remarks . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 27. Strain gradient plasticity . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 29. 2.2.1. Overview of strain gradient phenomena and previous models . . . . . . . . .. 31. 2.2.2. Problem formulation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 34. 2.2.3. Rate problems and deformation theory . . . . . . . . . . . . . . . . . . . . . .. 36. 2.2.4. Deformation theory of plasticity . . . . . . . . . . . . . . . . . . . . . . . . .. 38. 2.2.5. Energy growth properties . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 41. 2.2.6. The intrinsic length ` . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 43. 3 Optimal Scaling Laws in Ductile Fracture by Void Sheet Formation 3.0.7. Main result . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 48. 3.0.8. Lower bound . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 50. 3.0.9. Upper bound . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 58. 4 Physical Interpretation and Experimental Validation 4.1. 4.2. 47. 70. Physical interpretation . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 70. 4.1.1. Cohesive-energy interpretation . . . . . . . . . . . . . . . . . . . . . . . . . .. 71. 4.1.2. Relation to Jc . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 72. Comparison with experiment . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 74. 5 Conclusion and Future Work. 78. 5.1. Summary . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 78. 5.2. Future work . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 80. Appendix A Non-local regularization. 81. Appendix B Non-local regularization : General case. 85. Bibliography. 87.

(11) xi. List of Figures. 1.1. Photomicrograph of a copper disk tested in a gas-gun experiment showing the formation of voids and their coalescence into a fracture plane [49]. . . . . . . . . . . . . . . . . .. 1.2. 2. Fracture surface in SA333 steel at room temperature and strain rate 3 × 10−3 s−1 . Taken from Kamat et al [60] . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 2. 1.3. Temperature dependence of the fracture energy of an A508 steel. Taken from [112] . .. 5. 2.1. Force-elongation curve for different values of n. . . . . . . . . . . . . . . . . . . . . . .. 18. 2.2. Plot of the function Φ used in the localization construction. . . . . . . . . . . . . . . .. 25. 2.3. Necking construction exhibiting localization on the central plane. The construction converges to fracture . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 2.4. Plastic strain gradients are caused by the geometry of deformation(a,b), by local boundary conditions (c,d) or by the microstructure itself (e,f). Source:[30] . . . . . . . . . .. 2.5. 27. 30. Torsional response of copper wires of diameter 2a in the range 12-170 µm. If the constitutive law were independent of strain gradients, the plots of normalized torque Q/a3 vs κa would all lie on the same curve. Source:[30] . . . . . . . . . . . . . . . . .. 2.6. 32. Schematic diagram of geometrically necessary dislocations underneath the indenter (Nix and Gao 1998,[90]) . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 35. 2.7. Depth dependence of the hardness of (111) single crystal copper. Source:[90] . . . . .. 35. 2.8. Schematic of kink formation (reproduced from [? ]). a) Slip strains γ ± = ± tan θ; b) rotations through ± tan θ. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 44.

(12) xii 3.1. Sketch of the deformation mapping u employed in the upper bound. The central layer of thickness 2a stretches to a thickness 2a+2δ. A number of voids, shown as dots in the reference configuration on the left and as shaded regions in the deformed configuration on the right, open in order to satisfy the volume constraint. . . . . . . . . . . . . . . .. 3.2. ∗∗ Sketch of the functions W and WM for p = 0.2 and M = 8. The marked points ∗∗ correspond to λ = 1, aM p , λp , M . The upper curve is W , the lower one WM . . . . . . .. 3.3. 55. Void growth within a cube of size 2a. Conservation of volume of the hatched areas is used to determine the functions h and k, see 3.0.56, 3.0.61. . . . . . . . . . . . . . . .. 4.1. 50. 60. Renormalized specific fracture energy Jc /J0 and bounds shown as a function of the hardening exponent n for nickel, iron, copper and aluminium alloys at temperature of 300K, 195K, and 76K (data from [131]). a) Dislocation wall model of `. b) Nix-Gao [90] model of `.. . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . . .. 74.

(13) xiii. List of Tables. 4.1. Table of experimental data for various materials at various temperatures. RT: room temperature. The values of K (strength coefficient) and n (hardening exponent, equal to p) were obtained by fitting the stain strain curves of the corresponding material. Impact toughness is expressed as the Charpy energy per unit of fracture area. Source: K. A. Warren and R. P. Reed, Tensile and Impact Properties of Selected Materials from 20 to 300K, Monograph 63, National Bureau of Standards, June 1963. . . . . . .. 77.

(14) 1. Chapter 1. Introduction 1.1 1.1.1. General overview Experimental observations. Ductile fracture is a fundamental failure mode of metals that results from a concatenation of microscopic mechanisms of deformation including void nucleation, growth, coalescence and, ultimately, localization into fracture planes, cf. Figure 1.1, cf. also [31], [127] and references therein. In structural materials, the voids nucleate mainly at inclusions and second phase particles, by decohesion of the particle-matrix interface or by particle cracking (Goods and Brown 1979 [44], Puttick 1959 [94]), and subsequent void growth is driven by the plastic flow around the surrounding matrix. Unlike brittle materials, ductile materials undergo extensive plastic deformation before reaching the final stage of fracture. Tensile experiments on rounds bars often reveal that the failure is preceded by an important flow localization process characteristic of necking. Indeed, it is a common observation that necking comes with a substantial reduction in the cross sectional area, and further plastic deformation requires less applied stress. As a consequence, typical engineering stress-strain curves go through a maximum, sometimes identified as the Ultimate Tensile Strength (UTS) or onset of necking, a process which is followed by a geometrical softening until final separation of the specimen. As a result, the total work of fracture is ostensibly much larger in ductile materials than brittle materials, the excess being attributed to the plastic dissipation. The evidence that void growth and coalescence represents the major failure mechanism in most.

(15) In this simulation of a gas-gun experiment, (a) is the initial configuration of aluminum striking a copper target, and (b) shows formation of spall. The green area on the left is the aluminum plate that strikes a 5-millimeter-thick cylindrical disk target. The target’s two spall rings can be seen on the disk. The formation of voids (red) is seen in the center of the disk.. 2. material, which closes the voids created by the original shock. Under these conditions, the damaged material could jet out from pores, continue deforming, have localized heating, and even melt.. This photomicrograph of a copper disk used in a gas-gun experiment shows the formation of voids in the spall layer.. Figure 1.1: Photomicrograph of a copper disk tested in a gas-gun experiment showing the formation of voids and their coalescence into a fracture plane [49].. Lawrence Livermore National Laboratory. Figure 1.2: Fracture surface in SA333 steel at room temperature and strain rate 3 × 10−3 s−1 . Taken from Kamat et al [60] structural materials comes from fractography studies using Transmission Electron Microscopy. These studies reveal that the fracture surfaces contain spherical dimples, which represent microvoids, cf. Figure 1.2. This is in stark contrast to the sharp specular cracks that result from brittle fracture. Ductile fracture is of particular importance for industrial applications (oil and gas pipelines, nuclear powerplants, etc.) and the determination of fracture properties of ductile materials has been the focus of numerous investigations. In particular, a certain number of testing standards have been put forth, that, in turn, provide the basis for experimental design of materials. Among these testing standards, two require specific attention: J-testing and Impact testing..

(16) 3. 1.1.2. J -integral testing. J -testing, which has been widely used in fracture mechanics, expresses the fracture criterion as a critical value of the J -integral. The standard JIc Test Method, E 813, has been issued by ASTM for determining the plane strain value of J at initiation of crack growth, namely JIc . The value of JIc obtained by this method may be used to characterize the toughness of materials at the onset of crack extension. The method originates from the observation of Begley and Landes [11] that J can be experimentally determined by the energy released rate according to the relation. J =−. 1 ∂U ( )∆ B ∂a. (1.1.1). where U is the strain energy and B is the thickness of the specimen. For a given value of ∆, one can use multiple specimens with different crack lengths a to compute the load-displacement curve. The area under this curve therefore represents the total strain energy, which can then be plotted as a function of the crack length. The value of J is retrieved from taking the negative slope of the strain energy versus crack length curve. The procedure could be repeated for different values of ∆ to obtain a curve J versus ∆. Evidently, this method requires the use of multiple specimens and therefore has been improved in order to estimate J from a single measure load-displacement curve, as proposed by Rice et al [99]. More specifically, the standard JIc testing procedure, which uses a three point bend specimen and a compact specimen, requires the measurement of applied load and load-point displacement to obtain the total work done on the specimen. The load versus displacement is recorded automatically by an X-Y recorder and the extensions of the crack length are measured after breaking up the specimen upon deforming the specimen to desired values. The values of J are plotted against the crack growth to obtain an R-resistance curve which is fitted through a linear regression line. The critical JIc is then determined by the intersection between this line and the blunting line defined by J = 2σy ∆ap. (1.1.2).

(17) 4 where σy represents the yield stress and ∆ap the physical crack extension. The use of the blunting line in equation (1.1.2) refers to the crack growth due to crack-tip blunting. It bears noting that this testing procedure additionally assumes specific validity conditions on the geometry of the specimen, as explained in the comprehensive study of fracture mechanics presented in Kanninen and Popelar [61]. Further details about the procedure have been skipped in this overview, but the reader can find a more extensive review of the method in [61]. This standard testing approach has found important applications in the characterization of a wide range of ductile engineering materials.. 1.1.3. Impact testing. Impact testing measures the energy required to break a material sample. On the contrary of J testing, the fracture energy obtained cannot be formally put into an equation. The most standard impact test is the Charpy V notch impact test which consists of a specimen containing a 2mm deep notch with radius 0.25mm. The specimen, treated at a desired temperature, is placed into a holder and then struck with a hammer. The hammer is mounted at the end of a pendulum which is adjusted so that its kinetic energy is 240f t − lb when it hits the specimen. Upon breaking of the bar, the hammer reaches a final height, and the difference between the initial height and the final height translates into the energy absorbed by the material sample during the breaking. This energy is measured as the fracture energy of the material. This method has been extensively used to characterize fracture properties of materials at diverse temperatures and it has been observed that the specific fracture energy increases as a function of the temperature, which in turn, suggests that different fracture mechanisms occur at low temperatures and high temperatures. Figure 1.3 shows a typical Charpy curve obtained from a French A508(16M N D5) steel broken at various temperatures and strain rates. This picture illustrates a complex dependence of the fracture energy on temperature and reveals that at high temperatures, A508 steels fail by microvoid coalescence, characteristic of ductile failure whereas at low temperatures, they undergo cleavage fracture. This leads to the existence of a transition temperature at which the material behavior goes from brittle to ductile, and such temperature often receives the name of Ductile to Brittle Transition Temperature.

(18) 5. 250 . Energy CVN (J). 200. . m.s m.s m.s . 150 100. . 50. hal-00142084, version 1 - 23 Apr 2007. 0 -200. -150. . -100. -50 0 Temperature ( C ). 50. 100. Fig. 4. Charpy V–notch (CVN) fracture toughness transition curves of 16MND5 (A508) for T–L Temperature Charpy specimens tested at different loading rates. Figure 1.3: dependence of the fracture energy of an A508 steel. Taken from [112]. (DBTT). In general, the temperature and strain rate dependence of fracture properties of materials has been the subject of scientific investigation, see for instance Kamat et al [60], Tvergaard and Needleman [128], Shin et al [106], Shetty et al [105], Armstrong and Walley [3], Wang et al [130], and references therein.. 1.1.4. Surface energies. We summarize here two major mechanisms responsible for the surface energies in ductile fracture: the coalescence of cavities by internal necking and the cleavage crack growth in presence of plastic deformation. In Thomason 1970 [120], an estimate of the surface energy for the coalescence of cavities was derived. The results suggested that internal microscopic necking of ligaments between cavities contributes to the total surface energy and that the corresponding surface energy is a function of the mean-free-path between cavities or second phase particles. The model used a coalescence criterion derived in Thomason 1968 [119] to compute the plastic work per unit area of subsequent fracture. 32 surface during necking down, i.e. when the the cross sectional area of the ligaments is further reduced after a uniform extension. The theoretical values of the coalescence energy obtained were.

(19) 6 found to be about an order of magnitude less than experimental estimates of the total surface energy for ductile crack propagation. In reality, experimental measurements include a contribution from pre-coalescence straining ahead of the advancing crack which strongly depends on the extent of the plastic zone ahead of the crack. Plastic dissipation around a crack tip supplies a considerable contribution to the fracture energy in ductile materials. The surface energy associated with crack growth is related to the microscopic mechanisms of cleavage in the presence of plastic flow. A wealth of experimental evidence exhibited the phenomenon of crack propagation in the presence of pre-existing dislocations. For example, it was found in Lipkin et al, [71] that a sharp crack can propagate along a gold-sapphire interface, nevertheless the gold deforms plastically, indicating the motion of vast quantities of dislocations and the measured fracture energy was found to be orders of magnitude larger than the surface energy. When fracture occurs by atomic separation, the length scale of the fracture process is typically smaller than the dislocation spacing or the elastic cell size within the dislocation structure, which is the length scale of the plastic deformation. Thus, in a small region near the tip, the stress fields are more like those at a linear elastic crack tip singularity. Because of the large disparity between relevant length scales involved in plastic flow processes around cracks in metals and metal-ceramic interfaces [110], Suo et al, [110] have proposed the use of a long dislocation free strip of elastic material inside which the crack propagates. These lengths typically consist of the Burgers vector, b ∼ 10−10 m which is relevant for fracture by atomic separation; the nominal dislocation spacing, around 10−7 − 10−6 m, characteristic of plastic flow; and the overall plastic zone size. A similar approach using an elastic strip was further used by Beltz et al, [12] to develop a self-consistent model for cleavage. Basically, the idea is to postulate that the crack tip does not emit any dislocation and there exists a core elastic region (i.e. free of dislocations) near the tip surrounded by the plastic zone. Using finite element calculations, it was found that, in order for a steady-state crack growth to occur, the applied energy release rate must generally be several orders of magnitude larger than Griffith energy at the crack tip (i.e. inside the elastic strip). This result is well in agreement with experimental observations, e.g. Tetelman [116], which suggest that the fracture energy is expected to be up to 4 orders of magnitude.

(20) 7 larger than surface energies.. 1.2. Previous work on ductile fracture. The first micromechanical studies of ductile fracture go back to the pioneer works of McClintock 1968 [77] and Rice and Tracey 1969 [98] who studied the growth of a single void in an infinite elasticplastic solid, and showed that fracture by void coalescence is promoted by a high level of stress triaxiality. This was confirmed by numerous triaxial tension test experiments on tensile specimens (Hanckok and Mackenzie 1976 [48], Hancock and Brown 1983 [47]). Gurson 1977 [45] developed the most widely known porous ductile material model based on averaging techniques. His void growth model was given in terms of a macroscopic yield condition as a function of one microstructural parameter, namely the void volume fraction. A number of extension models have been attempted in order to account for void nucleation (Chu and Needleman 1980 [16]), void shape effects (Gologanu, Leblond and Devaux [37], [39], [41], [43]), strain hardening effects (Leblond et al 1995 [70]), kinematic hardening (Mear and Hutchinson 1985 [79]). Also, computational models have been put forth to investigate the void growth and coalescence mechanism. Such micromechanical models, sometimes referred to as cell model studies, have been the focus of numerous authors such Tvergaard [121], [124], [126],[125], Hutchinson and Tvergaard 1987 [58], Needleman and Tvergaard 1984 [88]. Coalescence models also include the studies of Gologanu [38], [40], [42] or Thomason [119], [117], [118]. During the deformation of ductile solids, it is observed that a smooth deformation can develop into a highly concentrated deformation pattern, which corresponds to the localization of the plastic flow into shear bands. Analysis of the bifurcation into shear bands has been the subject of the works of Hill 1962 [52], Rice 1977 [96], and Rudnicki and Rice 1975 [100]. A wealth of computational description of plastic localization is contained in the works of Tvergaard [121], [124], [126],[125]. Those treatments, which complement the initial void model of Gurson, mainly revealed the presence of voids as main catalysts of localization and derived critical coalescence conditions. Recently, efforts have been made to relate macroscopic properties to the structure and material behavior at the microscale. For instance, Pardoen and Hutchinson 2002 [93] developed relations.

(21) 8 between fracture toughness and microstructural details for ductile materials based on a generalized Gurson model that accounts for both growth and coalescence. The microstructural parameters were the initial porosity, the void shape and spacing, as well as the void spacing anisotropy. In the works of Tvergaard ([126],[122], [123],[89]) and Nielsen and Tvergaard [89], an emphasis has been on the interaction between voids with two size length scales, the smaller size voids appearing as defects in the ligaments, i.e. spacing between primary voids.. 1.3. Motivation. So far, the existing experimental data at best provide partial coverage of ductile fracture properties over a limited range of temperatures, strain rates and other relevant operating conditions, and may be entirely lacking under off-normal or extreme conditions and for new materials. The existing micromechanical models, which strongly rely on conventional plasticity theories, partially explain the complex dependence of the fracture properties on temperature and strain rate. Moreover, models that accurately quantify surface energies and rigorously predict their contribution to the total work of fracture are still almost non existent. Finally, the classical models (mostly empirical or computational) rely strongly on heuristics and intuition and often do not lend themselves to a mathematically rigorous analysis of ductile fracture. The goal of this thesis is to present a rigorous mathematically tractable model that unifies plasticity, surface energy and fracture. An emphasis will be put on the complex relationship between macroscopic quantities and microscopic properties, along with their temperature dependence, within a multiscale framework. In this way, the present work describes ductile fracture as a multiscale phenomenon, and therefore falls naturally within a multiscale hierarchy. The multiplicity of length scales involved in ductile fracture strongly suggests the use of methods of multiscale analysis from the calculus of variations. Indeed, despite the irreversible and pathdependent character of plasticity, under monotonic and proportional loading conditions plasticity problems may be recast as energy minimization problems by recourse to deformation-theory of plasticity (e. g., [75] and references therein). Throughout this work, we therefore assume deformation.

(22) 9 theory of plasticity and by effective energy we specifically mean a deformation-theoretical energy that jointly accounts for both free energy and plastic dissipation. Two main features render the resulting ductile-fracture problem non-standard and lend it mathematical interest, namely, sublinear energy growth and strain-gradient hardening. The physical basis underlying these fundamental properties may be understood as follows. For large material samples undergoing slowly-varying deformations in their interior, the effective energy of metals is observed to ostensibly exhibit conventional volume scaling, i.e., it scales with the volume of the sample when all lengths, including displacements, are scaled uniformly. Energies that possess volume scaling are referred to as local, since they can be written as the integral of an energy density which depends on the local deformation gradient. Such local energies can be characterized by means of conventional constitutive testing, such as uniaxial tension tests, tension-torsion tests, and other similar means. However, when observed through constitutive tests on large samples, the local limit of the effective energy of metals is invariably found to exhibit sublinear growth at large deformations (cf. section 2.1.1). Such sublinear growth is a reflection of the work hardening characteristics of large metallic specimens and gives rise to well-known geometric instabilities such as the necking of bars, sheet necking, and others (cf., e. g., [76]). From the viewpoint of the calculus of variations, energies with sublinear growth relax to zero for every deformation and thus fail to supply useful information regarding the fracture properties of metals. Physically, the relaxation process corresponds to the concentration of deformation to small volumes such as shear bands. The deformation is then proportional to 1/δ in a volume of size δ → 0, and since the energy density has sublinear growth its contribution to the total energy is negligible in the limit. Similar instabilities are present in many local problems characterized by nonconvex energy densities. In metals undergoing ductile fracture this inherently unstable behavior is held in check by a second fundamental property of metals, namely, the strain-gradient hardening [27, 30, 28, 29]. This property of metals has been extensively investigated and demonstrated by means of torsion tests in wires [30], nanoindentation [90, 132, 54], and by other means. Specifically, for fixed local deformation, the effective energy density of metals is observed to be an increasing function of the local strain.

(23) 10 gradient, or the second deformation gradient. This property results in deviations from volume scaling, i.e., in nonlocal behavior and size dependency, in sufficiently small material samples. Under these conditions, we show in the present work that ductile fracture emerges as the net result of two competing effects: whereas the sublinear growth of the energy in the large-body limit promotes localization of deformation in large samples to failure planes, the size-dependence of metal plasticity stabilizes this process of localization in its advanced stages, thus resulting in an orderly progression towards failure and a well-defined specific fracture energy.. 1.4. Outline of the thesis. The plan of the thesis is as follows: The last section of this introductory chapter is devoted to some mathematical preliminaries. We present basic concepts from topology and functional analysis, and define notations that will be used throughout the thesis. In Chapter 2, we show that homogenization fails for ductile fracture. More precisely, we show explicitly, by means of a simple construction, later referred to as a necking construction, that the sublinear growth of the energy density is responsible for the localization of deformations. The strain energy then relaxes to zero, which evidently provides no useful information on fracture properties. This motivates the addition of a stabilizing non-local component to the strain energy density that accounts for size effects using strain gradient plasticity. As a consequence, a characteristic length scale is introduced, in the same spirit of previous strain gradient plasticity models in the literature, which will briefly be discussed as well in this chapter. We present a simple deformation theory of plasticity model that accounts for both local and non-local effects. The aim of Chapter 3 is to present a rigorous analysis of some qualitative properties of ductile fracture. The key strategy consists of the derivation of optimal scaling laws—as opposed to searching for exact minimizers—for energies exhibiting both sublinear growth in the local limit and straingradient hardening. The main result is that optimal scaling is achieved by a void sheet construction and the fracture energy obeys a well- defined relationship with respect to other material parameters,.

(24) 11 namely the imposed displacement, the length scale and the hardening exponent. Physical interpretation and experimental validation are the core of Chapter 4. On the one hand, we derive a physical explanation of the optimal scaling laws of Chapter 3. On the other hand, we assess the validity of the scaling relations based on experimental data. We show that the test data collapse remarkably within the bounds predicted by the analysis. We present our concluding remarks and future directions as part of Chapter 5. We particularly evoke some aspects of the numerical implementation using finite elements.. 1.5. Mathematical Preliminaries. We present some basic concepts of functional analysis and topologies associated with function spaces. Throughout this work, the notation “D” will be used to denote the gradient. We start with the definition of the classical Lebesgue spaces Lp . Definition 1.5.1 (Lebesgue spaces) (i) Let Ω ⊂ Rn be an open set and 1 ≤ p ≤ ∞. For u : Ω → R, we set:. Z kukLp := ( |u|p dx)1/p if 1 ≤ p < ∞ Ω. kukL∞ := inf {C ∈ [0, ∞] : |u(x)| ≤ C f or a.e. x ∈ Ω}. We say that u ∈ Lp (Ω) if kukLp (Ω) < ∞. The set Lp (Ω) is a Banach space and k.kLp is a norm on that space. (ii) Let un , u ∈ Lp (Ω). We say that un → u strongly in Lp if kun − ukLp → 0 as n → ∞. As illustrated in Definition 1.5.1, the definition of the Lebesgue space does not involve first or higher order derivatives. Derivatives are accounted for by extending the concept of norm Lp to u and its derivatives, which gives rise to Sobolev spaces. Definition 1.5.2 (Sobolev spaces) Let Ω ⊂ Rn be an open set and 1 ≤ p ≤ ∞. We define the Sobolev space W 1,p (Ω) by the set of functions u : Ω → R, u ∈ Lp (Ω), whose weak partial derivatives.

(25) 12 ∂u ∂xi. ∈ Lp (Ω) for every i = 1, .., n. We endow this space with the following norm. kukW 1,p := (kukpLp + kDukpLp )1/p if 1 ≤ p < ∞ kukW 1,∞ := max{kukL∞ , kDukL∞ } if p = ∞. Strong connections between Lebesgue spaces, Sobolev spaces and their topologies are reflected through the Sobolev embedding theorem and Sobolev inequalities, whose statements and complete proof can be found in [26]. Here we simply recall the classical Sobolev inequalities, also referred to as Poincaré inequalities. Theorem 1.5.1 Let Ω ⊂ Rn be a bounded open set with a Lipschitz boundary. (i) Case 1. If 1 ≤ p < n, then W 1,p (Ω) ⊂ Lq (Ω) for every q ∈ [1, p∗], where p∗ is the Sobolev exponent defined by 1 1 np 1 = − , i.e. p∗ = p∗ p n n−p. (1.5.1). More precisely, for every q ∈ [1, p∗] there exists c = c(Ω, p, q) such that. kukLq ≤ ckukW 1,p. (1.5.2). (ii) Case 2. If p = n, then W 1,n (Ω) ⊂ Lq (Ω) for every q ∈ [1, ∞). More precisely, for every q ∈ [1, ∞) there exists c = c(Ω, p, q) such that. kukLq ≤ ckukW 1,n. (1.5.3). For more details concerning Sobolev spaces, we refer to Adams [1], Brezis [13], Dacorogna [21], Dacorogna-Marcellini [22], Ekeland-Temam [25], Evans [26], Gilbarg and Trudinger [35], Giusti [36], Kufner-John-Fucik [65], Ladyzhenshaya-Uraltseva [69] or Morrey [84]. We finish this section with a brief overview of functions of bounded variation. Functions of bounded variations (BV functions) have an important application for problems in the calculus of.

(26) 13 variations. This class of functions has been the natural tool to study problems characterized by free discontinuities, for example image segmentation theory or fracture mechanics. BV functions have two main characteristics: they are functions with a measure distributional derivative or function which are L1 limits of of bounded sequences in W 1,1 . In what follows, we present some of the basic definitions and results, taken from the book of Ambrosio, Fusco and Pallara [2]. We refer the reader to this book for a thorough description of BV spaces. Definition 1.5.3 Let u ∈ L1 (Ω); we say that u is a function of bounded variation in Ω if the distributional derivative of u is representable by a finite Radon measure in Ω, i.e. if. Z u Ω. ∂φ dx = − ∂xi. Z. φ dDi u ∀φ ∈ Cc∞ (Ω), i = 1, ..., N. (1.5.4). Ω. for some RN -valued measure Du = (D1 u, ..., DN u) in Ω. The vector space of all functions of bounded variation in Ω is denoted by BV (Ω) An equivalent representation of the formulae in 1.5.3 is:. Z u divφdx = − Ω. N Z X i=1. φi dDi u ∀ φ ∈ [Cc1 (Ω)]N. (1.5.5). Ω. An important observation is that the Sobolev space W 1,1 (Ω) is contained in BV (Ω), because its directional derivative is absolutely continuous with the standard Lebesgue measure of RN , with a Radon-Nikodym derivative corresponding to the (approximate) gradient of u, see [2]. An advantage of BV spaces is that, unlike Sobolev spaces, they include characteristic functions of sufficient regular sets, and more generally piecewise smooth functions. Now, we proceed to the definition of the variation of BV functions, which provides an equivalent characterization of BV spaces. Definition 1.5.4. (i) Let u ∈ [L1loc (Ω)]m (locally integrable). The variation V (u, Ω) is defined by N Z X V (u, Ω) := sup{ uα divφα dx : φ ∈ [Cc1 (Ω)]n×N , kφk∞ ≤ 1} i=1. Ω. For u continuously differentiable, then V (u, Ω) =. R Ω. |Du|dx.. (1.5.6).

(27) 14 (ii) Let u ∈ [L1 (Ω)]m . Then u belongs to [BV (Ω)]m if and only if V (u, Ω) < ∞. In addition, V (u, Ω) = |Du|(Ω) for u ∈ [BV (Ω)]m , here |Du|(Ω) represents the total variation of the measure Du. (iii) The space [BV (Ω)]m endowed with the norm. Z kukBV :=. |u|dx + |Du|(Ω). (1.5.7). Ω. is a Banach space. Now we introduce the so-called weak* convergence in BV (Ω), which is weaker than the norm convergence. Definition 1.5.5 (Weak* convergence) Let u, un ∈ [BV (Ω)]m . We say that (un ) weakly* converges in [BV (Ω)]m to u if (un ) converges to u in [L1 (Ω)]m and (Dun ) weakly* converges to Du in measure in Ω, i.e. Z n→∞. Z φ dDu ∀ φ ∈ C0 (Ω). φ dDun =. lim. Ω. (1.5.8). Ω. A simple criterion for weak* convergence is given by the following proposition (see [2], Proposition 3.13) Proposition 1.5.1.1 Let (un ) ⊂ [BV (Ω)]m . Then (un ) converges weakly* to u in [BV (Ω)]m if and only if (un ) is bounded in [BV (Ω)]m and converges to u in [L1 (Ω)]m . The concepts above mentioned are useful for the analysis presented in Chapter 2 and Chapter 3 of this thesis..

(28) 15. Chapter 2. From Necking Instability to Strain Gradient Plasticity In this chapter, we wish to argue that conventional plasticity models do not suffice to understand ductile fracture, and thus, one has to introduce non-local effects, which naturally suggests the existence of a characteristic length scale. The key point to this observation is that, from the standpoint of the calculus of variations, the energy densities are concave due to their sublinear growth (see section 2.1.1), and thus their corresponding energy functionals relax to zero. We illustrate this concept by means of a simple example, which mainly serves as a motivation for formulating a strain gradient plasticity model. The relaxation is achieved by a localization technique suitable for non-convex problems.. 2.1. A localization construction. In conventional theories of plasticity, large material samples exhibit energies that have a volume scaling, i.e. energies scale as the volume of the sample when all lengths, including the displacements, are scaled uniformly. Such energies are referred to as local and are appropriate to describe plasticity for bulk materials. Local theories derive mostly from conventional constitutive testing, e.g. uniaxial tension experiments, which provide the basis for constitutive laws, which in turn, can be recast in the form of energy functionals by recourse to the deformation theory of plasticity. For large deformations, the energies possess a sublinear growth that is a reflection of the work hardening.

(29) 16 characteristic of large metallic specimen and gives rise to geometric instabilities such as necking. In this section, we present an analytical description of necking and how it relates to localization of plastic deformation which usually precedes fracture in ductile materials.. 2.1.1. Uniaxial tension test. Let Ω ∈ R3 be a bounded domain undergoing a transformation u : Ω → R3 . Within the context of deformation theory of plasticity, the bulk energy density of crystalline materials results from the contribution of both an elastic energy and a plastic stored energy according to the relation:. W (F, Fp ) = W e (F Fp−1 ) + W p (Fp ). (2.1.1). where F = Du and Fp represents the plastic transformation. We have used the the multiplicative decomposition F = Fe Fp . The incompressibility of the plastic transformation yields the additional constraint detFp = 1. (2.1.2). Consider the uniform uniaxial tension (along the x3 direction) of a rigid-plastic bar for which the deformation gradient is homogeneous and given by F = Du = diag( √1λ , √1λ , λ). We further assume that the material undergoes a fully plastic deformation, in which case Du = Fp . The energy density then reads: W (F ) = W p (F ). (2.1.3). We have assumed the material to be rigid plastic, i.e W e vanishes in SO(3). The incompressibility condition further reduces to detF = 1. (2.1.4). For crystalline materials, stress-strain curves exhibit a power-law relationship between the true stress and the engineering strain in the form σ = K(λ − 1)n where K is the strength coefficient and n is the hardening exponent, with 0 < n < 1 for metals. Then the Piola-Kirchhoff stress P , which is.

(30) 17 equal to the axial force applied to the rod divided by the undeformed cross-sectional area, is given by: P = ∂λ W = K(λ − 1)n λ−1. (2.1.5). ∂λ W ∼ Kλn−1. (2.1.6). which for large λ scales as. Therefore, in the same range the energy density scales as. W ∼. K n λ n. (2.1.7). K n. (2.1.8). Now let us denote for the rest of the sequel. A=. We take the previous assumptions as grounds for defining a bulk energy functional of the form:. Z Ebulk (u) = A. (|Du|n − 3n/2 )dx. (2.1.9). Ω. The term 3n/2 guarantees that the stored energy is zero when Du = I, where I is the identity matrix. A simple dimensional analysis shows that the quantity A is in the unit of a pressure (Pascal) which corresponds to an energy per unit volume. Conformably to (2.1.9), the strain energy density satisfies. W (F ) ∼ |F |n. (2.1.10). with 0 < n < 1. Because the exponent n < 1, the strain energy density W is said to have a sublinear growth. For the homogeneous deformation considered in this section, the bulk energy reads:. Ebulk (λ) = A|Ω|((λ2 +. 2 n/2 ) − 3n/2 ) λ. (2.1.11).

(31) 18 where |Ω| represents the volume of the domain Ω. The Piola stress then reads:. P (λ) =. 2 n ∂W 1 = An(λ − 2 )(λ2 + ) 2 −1 ∂λ λ λ. (2.1.12). Figure 2.1 illustrates the dependence of the force P as function of the elongation for different values of n. It is clear from the plot that for n ≥ 1, the force increases continually with the elongation, but this behavior is different when n < 1, the range for most metals. Indeed, the curve shows an increase of the force versus elongation up to a maximum value, and subsequent elongation requires less applied force. This decrease of the force with respect to the elongation for sufficient large elongations is characteristic of geometrical softening, a fundamental property of ductile materials. Such behavior is mainly tied to the sublinear growth of the energy density and confirms the Considère prediction [17] that necking is more likely to occur for materials whose force-elongation curves go through a maximum.. 2. n=1.2. P( λ ). 1.5. n=1.0. 1. n=0.8. 0.5. 0. 0. 2. 4. λ. 6. 8. 10. Figure 2.1: Force-elongation curve for different values of n..

(32) 19. 2.1.2. Necking construction. In this section, we provide an analytical, but simple characterization of plastic localization, by means of a simple example. We consider here a bar with square cross-sectional area, clamped at its bottom and subject to a prescribed displacement on its top. Within the assumptions of section 2.1.1, we wish to minimize the quantity (2.1.9). More precisely, we consider the minimum problem:. Z inf {Ebulk (u) = A. (|Du|n − 3n/2 )dx : detDu = 1}. (2.1.13). Ω. The infimum value for (2.1.13) is zero and is achieved by a minimizing sequence that exhibits concentration on the mid-plane, as stated in the following proposition: Proposition 2.1.0.2 Let Ω = {(x1 , x2 , x3 ), − a2 ≤ x1 ≤. a a 2,−2. ≤ x2 ≤. a 2 , −L. ≤ x3 ≤ L}. The bar. is subject to uniaxial axial tension along the x3 axis and the boundary conditions are expressed as follows: u3 (x1 , x2 , −L) = −L. (2.1.14). u3 (x1 , x2 , L) = L + δ Let Φ : [−L, L] → R continuous and compactly supported on [−L, L] defined by:. Φ(x3 ) =. . δ x3 L( L. . x3 δ L (− L. + 1), + 1),. if − L ≤ x3 ≤ 0. (2.1.15). if 0 ≤ x3 ≤ L. Now consider the following sequence un of deformations: u1n = √ x0 1 ϕn (x3 ) u2n = √ x0 2 ϕn (x3 ) u3n = ϕn (x3 ). (2.1.16). where ϕn : [−L, L] → R is a sequence of continuous functions such that. ϕ0n (x3 ) = λn (x3 ) = 1 + nΦ(nx3 ). (2.1.17).

(33) 20 Then the following holds: (i) lim Ebulk (un ) = 0 n→∞. (ii) un converges weakly* to u in BV (Ω, R3 ) where u1 = x1 u2 = x2 u3 = ϕ(x3 ) with ϕ(x3 ) =. proof 2.1.1. (2.1.18). x3 ,. −L ≤ x3 ≤ 0. x3 + δ,. 0 ≤ x3 ≤ L,. (2.1.19). (i) We prove part (i). In order to avoid confusion of notation, the growth exponent. is denoted p instead of n which will be used to label any given sequence. Denoting ϕ0n (x3 ) = λn (x3 ), the deformation gradient is given by : Dun = . −1/2 λn (x3 ). 0 0. 0. −3/2 − 21 λn (x3 )λ0n (x3 )x1. . −1/2 1 −3/2 0 λn (x3 ) − 2 λn (x3 )λn (x3 )x2 , 0 λn (x3 ). (2.1.20). The sequence λn such defined is compactly supported in [−L/n, L/n] and the resulting sequence of maps exhibits a concentration effect on the plane x3 = 0. More precisely, the sequence λn is defined by:. λn (x3 ) =. 1, 1 + n δ (n x3 + 1), L L 1 + n Lδ (−n xL3 + 1), 1,. −L ≤ x3 ≤ −L/n −L/n ≤ x3 ≤ 0 0 ≤ x3 ≤ L/n L/n ≤ x3 ≤ L,. (2.1.21).

(34) 21 It follows that the corresponding sequence of maps can be expressed in the following form: un1 = √ x0 1 ϕn (x3 ) un2 = √ x0 2 ϕn (x3 ) un = ϕn (x3 ) 3 where. ϕn (x3 ) =. (2.1.22). x3 , 2 x3 + n δ (n x3 + x3 ) + δ , L 2L 2. −L ≤ x3 ≤ −L/n −L/n ≤ x3 ≤ 0. (2.1.23). x2 x3 + n Lδ (−n 2L3 + x3 ) + 2δ , 0 ≤ x3 ≤ L/n x3 + δ, L/n ≤ x3 ≤ L,. In what follows we wish to compute the following quantity. Ê = lim Ebulk (un ). (2.1.24). n→∞. A straightforward computation shows that:. 2 x2 + x22 λ02 n 1/2 + 1 ] λn 4 λ3n. (2.1.25). p/2 2 x2 + x22 λ02 n [λ2n + + 1 − 3p/2 )dx1 dx2 dx3 3 λ 4 λ n −L n. (2.1.26). |Dun | = [λ2n +. The bulk energy is given by:. Z. a 2. Z. a 2. Ebulk (un ) = −a 2. −a 2. Z. L. We can write that:. Z. L. −L. (λ2n +. 2 r2 λ02 n p/2 + ) dx3 = 2 λn 4 λ3n Z +. Z. −L/n. 3p/2 dx3. −L 0. (λ2n +. 2 x2 + x22 λ02 n p/2 + 1 ) dx3 λn 4 λ3n. (λ2n +. 2 x2 + x22 λ02 n p/2 + 1 ) dx3 λn 4 λ3n. −L/n. Z + 0. L/n.

(35) 22 Now let 0. Z. (λ2n +. 2 x2 + x22 λ02 n p/2 ) dx3 + 1 λn 4 λ3n. (2.1.27). (λ2n +. 2 x2 + x22 λ02 n p/2 ) dx3 + 1 λn 4 λ3n. (2.1.28). I1 = −L/n. And similarly let L/n. Z I2 = 0. Using the inequality (a + b)p/2 ≤ ap/2 + bp/2 for a, b > 0, p/2 < 1 we can write:. Z. 0. λpn dx3 + 2p/2. I1 ≤. By a change of variable u = 0. Z. x3 δ L (n L. x21 + x22 p/2 ) 4. Z. 0. −L/n. |λ0n |p 3p/2. λn. dx3. (2.1.29). + 1) we have the following equalities:. 0. δ x3 (1 + n (n + 1))p dx3 L L −L/n δ Z L2 1 L = n(1 + nu)p du nδ n 0. λpn dx3 =. −L/n. λ−p/2 dx3 + ( n. −L/n. −L/n. Z. 0. Z. =. L2 (1 + nu)p+1 Lδ [ ]0 δn2 p+1. =. L2 1 δ ((1 + n )p+1 − 1) δ(p + 1) n2 L. =. (1 + n Lδ )p+1 L2 1 ( − 2 ) → 0 as n → ∞ f or p < 1. δ(p + 1) n2 n. (2.1.30). Similarly, Z. 0. λ−p/2 dx3 = n. −L/n. L2 1 nδ n. Z 0. δ L. n du (1 + nu)p/2. δ 1 −1 [ ]0L p −1 − 1 (1 + nu) 2. =. L δn2. =. L 1 1 (1 − ) → 0 as n → ∞. p δ( p2 − 1) n2 (1 + n Lδ ) 2 −1. p 2 2. (2.1.31).

(36) 23 Finally Z. 0. −L/n. |λ0n |p. dx3 = 3p/2. λn. δ p L2 L2p δn. δ L. Z 0. n2p du (1 + nu)3p/2. p. =. δ δ L2 −1 n2(p−1) 3p ]0L [ 2p 3p/2−1 L δ( 2 − 1) (1 + nu). (2.1.32). δp L2 n2(p−1) = 2p 3p (n2(p−1) − ) 3p L δ( 2 − 1) (1 + n Lδ ) 2 −1 → 0 as n → ∞ when p < 1 and p 6= 2/3.. For p = 2/3, the previous calculation resumes to evaluating. n2p−2. Z 0. δ L. δ n dx = n2p−2 [log(1 + nu)]0L 1 + nu. (2.1.33). → 0 as n → ∞. It follows that I1 → 0 as n → ∞. A similar calculation also shows that I2 → 0. Finally, we have shown that: lim Ebulk (un ) = 0. (2.1.34). n→∞. (ii) Now we turn to part (ii). In virtue of proposition 1.5.1.1, it is enough to show that un → u in L1 and. R Ω. |Dun |dx bounded. We have:. Z. L. |ϕn (x3 ) − ϕ(x3 )|dx3 −L. Z L/n δ x2 δ δ δ x23 + x3 ) + |dx3 + |n (−n 3 + x3 ) − |dx3 |n (n L 2L 2 L 2L 2 0 −L/n Z 0 Z L/n 2 nx x3 δ nx2 x3 δ | 23 + 2n + 1|dx3 + | − 23 + 2n − 1|dx3 2 −L/n L L 2 0 L L Z 0 Z L/n δ x3 δ x3 (n + 1)2 dx3 + (−n + 1)2 dx3 2 −L/n L 2 0 L Z 1 L v 2 dv → 0 as n → ∞ δn 0. Z = = = =. 0. In the last equality, we have used the change of variables v =. nx L. (2.1.35). + 1 and v = − nx L + 1.

(37) 24 respectively. It follows then that:. ϕn → ϕ strongly in L1 [−L, L].. (2.1.36). Besides, using appropriate change of variable, Z. L. |λ−1/2 − 1|dx3 = n. −L. 2L2 δn. Z. δ L. |(1 + nv)−1/2 − 1|dv. 0. (2.1.37). δ 2L2 2 = [v − (1 + nv)1/2 ]0L → 0 as n → ∞ δn n. i.e. λ−1/2 → 1 strongly in L1 [−L, L] n. (2.1.38). From (2.1.36) and (2.1.38) it follows easily that. kun − ukL1 → 0 as n → ∞. (2.1.39). un → u strongly in L1 (Ω, R3 ). (2.1.40). i.e.. Finally, the boundedness of. R Ω. |Dun |dx comes naturally from the same calculations as in the. proof of part (i) with p = 1, in which case the boundedness of I1 (and thus I2 ) strictly follows from (2.1.30), (2.1.31), and (2.1.32). This concludes the proof.. . The construction defined by the sequence un can be intuitively understood as follows. We assume the minimizers to belong to a class of deformation mappings of the form given by (2.1.16), which evidently satisfy the conservation of volume constraint and the boundary conditions. The deformation inside the bar is homogeneous everywhere, except in a layer of size , see Figure 2.3, in which the plastic deformation is concentrated. The size of the layer, which depends on the sequence label n, is chosen such as to decrease to zero when n goes to infinity. At the same time, the cross sectional area inside the layer undergoes a drastic decrease, as the deformation in the x1 and x2 directions are.

(38) 25 divided by. √. λn (see the expressions of u1n and u2n in (2.1.16)). To make things more explicit, the. sequence of stretches λn is defined by λn (x3 ) = 1 + nΦ(nx3 ), where Φ is compactly supported in L [−L, L]. In this way, λn is supported on the set [− L n , n ], i.e. the size of the layer undergoing large. amounts of deformation. The multiplicative factor n contributes to increase the intensity of the deformation in the localized region, thereby decreasing the cross-sectional area, which in the limit becomes restricted to a point. We illustrate this concentration mechanism in Figure 2.3. Intuitively, the construction should converge to a discontinuous map with a crack amplitude at the mid plane equal to the imposed displacement. This discontinuous map u is characteristic of fracture of the material and part (ii) of proposition 2.1.0.2 states that the proposed construction indeed converges to a crack as expected. More importantly, the analytical construction reveals that the infimum energy is equal to zero.. δ/L. -L. 0. L. x3. Figure 2.2: Plot of the function Φ used in the localization construction.. In order to glean insight into the choice of the function Φ(x3 ), we reason as follows. We seek to construct a sequence of smooth deformations whose strains (λn (x3 ) − 1) concentrate at the origin. This is achieved by a simple piecewise linear function vanishing exactly at x3 = −L and x3 = L as depicted in Figure 2.2. The slope of each linear portion is then determined by making the sequence of strains (λn (x3 ) − 1) localize at the origin and converge to singular measure (dirac delta) with 0. a jump equal to the amplitude δ. Recall that λn = ϕn , therefore if λn is proved to converge to a.

(39) 26 singular measure, the corresponding limit of ϕn will be discontinuous. More precisely, the limit of ϕn belongs to SBV , the Special function of Bounded Variation, see [2]. To be more precise, let φ ∈ C0 [−L, L]. It is clear that. Z. L. Z. L. λn (x3 )φ(x3 )dx3 =. Z. L/n. φ(x3 )dx3 +. −L. −L. nΦ(nx3 )φ(x3 )dx3. (2.1.41). −L/n. Then. Z. L/n. Z nΦ(nx3 )φx3 )dx3 =. −L/n. L. v Φ(v)φ( )dv → n −L. Z. L. Z. L. Φ(v)dv < δ0 , φ > . (2.1.42). Φ(v)φ(0)dv = −L. −L. i.e. ∗. λn * 1 L1 + (. Z. L. Φ(v)dv)δ0 weakly ∗ in measure.. (2.1.43). −L. Note that L1 represents the one dimensional Lebesgue measure and δ0 represents the delta Dirac measure at the origin. Now remark that, due to the discontinuity of ϕ(x3 ) see (2.1.19), its derivative is a measure, i.e. Dϕ = 1 L1 + δ δ0. Equating. RL −L. (2.1.44). Φ(v)dv and δ identifies the amplitude of the discontinuity at the origin to the imposed. displacement δ. This is achieved for Φ(0) =. δ L,. and thus makes the choice of Φ more concise and given. by (2.1.15), see Figure 2.2. The convergence of un to u follows naturally from this construction. For reasons of simplicity, we have chosen the weak* convergence in BV as the main topology of convergence. The physical meaning of the results of proposition 2.1.0.2 is thus clear. On the one hand, the optimization problem (2.1.13) is ill-posed, as it relaxes to zero and provides no information about fracture properties. The infimum is obtained by means of a construction that features localization of plastic deformation. This localization of plastic flow is mainly attributed to the sublinear growth of the energy density and characteristic of necking. On the other hand, the necking construction converges to a discontinuous map, see Figure 2.3, which strongly implies fracture at zero cost. This.

(40) 27. Localization zone. δ. 2L. ε→0. Figure 2.3: Necking construction exhibiting localization on the central plane. The construction converges to fracture. contradiction is often referred to as the necking instability . From the viewpoint of the calculus of variations, the instability results from the lack of convexity (or quasi-convexity more precisely) of the integrand in the energy functional, and therefore minimizing sequences have to develop either oscillations or concentrations. In light of the analysis presented so far, local theories solely are insufficient to describe ductile fracture in metals. Although they can predict localization, necking and explain geometrical softening, they fail to provide useful and complete characterization of ductile materials. However, in metals undergoing ductile fracture, this inherent unstable behavior of large material samples is held in check by a second fundamental property of metals, namely, the strain gradient hardening. In section 2.2, we introduce a non-local model which will be the grounds for the explanation of size effects and surface energies, and yield a new multiscale model for ductile fracture.. 2.1.3. Some remarks. In concluding this section, we make some additional remarks concerning the type of energy functionals given by (2.1.13). Such a model is analogous to energy minimization problems in finite deformation elasticity. The subject of existence of minimizers in non-linear elasticity has been the.

(41) 28 focus of tremendous research in the calculus of variations, starting with the pioneering work of John Ball, [7]. The problem under investigation is the minimization of the elastic energy. Z I(u) =. W (Du)dx. (2.1.45). Ω. for the special class of stored-energy functions W that can be expressed as convex functions of the determinant and all the minors of the deformation gradient, functions which are referred to as polyconvex. From a physical point of view, this class of functions satisfy not only the material frame indifference, but also the condition that it takes an infinite amount of energy to compress the material to zero, requirements that are proper to finite elasticity. From a mathematical standpoint, this class of functions facilitates the use of the direct methods in the calculus of variations to prove existence of minimizers. More precisely, the problem reduces to proving the weak continuity of the determinant and other minors of the deformation gradient. Ball was able to show the existence of minimizers when W satisfies suitable growth conditions such as: (i) W (F ) ≥ c|F |p , for some c > 0 and p > 3; (ii) W (F ) ≥ c(|F |p + |cof F |q ), for some c > 0, with p ≥ 2 and q > p/p − 1 or; (iii) W (F ) ≥ c(|F |p + |cof F |q + |detF |r ), for some c > 0, p ≥ 2 and q ≥ p/p − 1 and r > 1. Many refinements of Ball’s results exist in the literature and we refer the reader to Ball and Murat[8], Giaquinta, Modica and Soucek [73], Muller, Tang and Yan [104]. The structure of the energy functional used in (2.1.13) is identical to (2.1.45), but evidently the energy density does not satisfy the growth conditions above stated, which makes the direct methods fail for plasticity problems, especially due to the sublinear growth. Instead, one has to perform a relaxation procedure and this was the core of section 2.1.2. The extension of Ball’s results to finite plasticity has been less studied, i.e. finite elastoplasticity problems of the form Z Ebulk (u, Fp ) = Ω. [W e (DuFp−1 ) + W p (Fp )]dx. (2.1.46).

(42) 29 In previous sections, we had made additional assumptions, such as Du = Fp for the purpose of illustration. The main difficulty here arises from the multiplicative elastic-plastic decomposition Du = Fe Fp . This problem was first attempted by Mielke and Muller [82] who showed the existence of minimizers for sufficient mild growth conditions on the energy densities, at the expense of adding a stabilizing energy term that comes from dislocations. The use of the direct methods in this context strongly relied on the div-curl lemma, the cornerstone of the theory of compensated compactness, see [86],[87],[114],[113],[115], [24],[103], for the statement and many of its refinements. Without the addition of a dislocation energy, the minimum problem does not admit a solution and minimizing sequences develop microstructures or concentrations and we refer the reader to [102],[46],[74],[80],[81],[91] for more details about relaxation and microstructures. In the same spirit, we need to formulate a stabilizing energy, which will relate to size effects and non-local plasticity. This is the focus of the next section.. 2.2. Strain gradient plasticity. A large body of literature has emerged on non-local theories of plasticity to explain size effects observed in the macroscopic response of materials as a function of microstructural sizes. For instance, a widely known result is the Hall-Petch effect which states that the yield stress is inversely proportional to the square root of the grain size in nanocrystalline materials. Size effects can be attributed to the presence of strain gradients, see [27], [30], [28], [29], which make conventional plasticity models break down for phenomena that involve a characteristic length scale. It is well known that plasticity is driven by the motion of dislocations which multiply and entangle to cause strain hardening, a process in which continued plastic deformation increases the crystal’s strength. The storage of dislocations comes from two sources: (1) dislocations accumulate by random trapping to form statistically stored dislocations; (2) because of the geometry of the solid or the material inhomogeneity, gradients in the plastic strain result in the formation of geometrically necessary dislocations , see [30] and Figure 2.4. Direct evidence for the notion that geometrically necessary dislocations lead to enhanced hardening comes from the compression tests of Russell and Ashby [101], Brown and Stobbs.

(43) 30 [14], and other authors. This strain gradient hardening property of metals has also been extensively investigated and demonstrated by means of torsion tests in wires [30], nanoindentation [90], [132], [54], and by other means. In general, strain gradients are inversely proportional to the length scale at which deformation occurs. When the length scale associated with the deformation field is large, strain gradients are very small and hardening is caused by statistically stored dislocations. In this case, conventional theories of plasticity apply and there is no internal length scale. On the other hand, when the deformations are small enough, it becomes a necessity to introduce strain gradient effects in the constitutive laws.. Figure 2.4: Plastic strain gradients are caused by the geometry of deformation(a,b), by local boundary conditions (c,d) or by the microstructure itself (e,f). Source:[30].

(44) 31. 2.2.1. Overview of strain gradient phenomena and previous models. Numerous phenomena in plasticity that depend on strain gradients have been presented in [28]. These phenomena include, but are not limited to, torsion of thin wires, grain size effect on polycristalline yield strength, void growth and softening, cavitation instabilities, etc. Torsion experiments Figure 2.5, see [28], [30] revealed a systematic increase of torsional hardening with decreasing wire diameter which implied the existence of a characteristic length scale in the constitutive laws. A candidate for strain gradient plasticity law was proposed by Fleck and Hutchinson in which size effect enters the constitutive law through the postulate that stress depends on strain and strain gradient. The formulation is presented within the context of deformation theory of plasticity, which assumes no important path-dependant behavior and monotone loading. In their approach to develop a strain gradient law, Fleck and Hutchinson [28] postulated that the strain density energy is a function of the overall effective strain which is defined by :. E=. p 2e + `2 χ2e. (2.2.1). q where e is the second invariant of strain e = 23 ij ij , and an analogous definition for the curvature q 2 χe = 3 χij χij . The length parameter ` is introduced for dimensional consistency. A power-law dependance of the strain energy density w on the effective strain E has the form. w=. n E n+1 Σ0 ( ) n n+1 E0. (2.2.2). where Σ0 , E0 and the strain hardening exponent n are material constants. Then the uniaxial stress σ is related to the uniaxial strain via the relation. σ = Σ0 (. E 1/n ) E0. (2.2.3). Fleck et al [28] were able to calibrate and validate their coupled stress version of strain gradient plasticity to the experimental results on copper wires (Figure 2.5) and found that values of ` between.

(45) 32 2µm and 4µm matched experimental data.. Figure 2.5: Torsional response of copper wires of diameter 2a in the range 12-170 µm. If the constitutive law were independent of strain gradients, the plots of normalized torque Q/a3 vs κa would all lie on the same curve. Source:[30]. Bassani [9] proposed a strain gradient model based on the postulate that the non-local tangent modulus, which accounts for strain hardening in addition to the conventional strain hardening, can be defined by the relation: Et =. E pe 1 −1 `2 α2 ( ) n [1 + ]1/2 n 0 (0 + κep )2. (2.2.4). 0 represents the yield strain in uniaxial tension, n is the hardening exponent and ep is the effective plastic strain. The material length parameter ` has been introduced again for dimensional consistency. The parameter α represents the maximum derivative of the plastic strain, through which non-local effects enter the model and κ is a dimensionless constant. By choosing appropriate values for the parameters appearing in equation 2.2.4, a good agreement was found between the model and the experimental results on copper wires by Fleck et al (1994). This approach of strain gradient plasticity has been used in the computational works of Tvergaard and Niordson, see [129], to account.

(46) 33 for the presence of a length scale in the interaction between voids. Nanoindentation experiments, see [90] also exhibit the importance of size effects due to strain gradients. The increase of hardness when the indentation size decreases, especially in the submicrometer depth regime, is attributed to large strain gradients inherent in small indentations that lead to the formation of geometrically necessary dislocations. First developed by Stelmashenko et al [109], [108], and De Guzman et al [23], the model of geometrically necessary dislocations was used by Nix-Gao to describe the depth-dependance of the hardness of crystalline materials. Specifically, they considered the indentation by a rigid cone (see Figure 2.6). Geometrically necessary dislocations develop in order to accommodate the indentation and the permanent shape change at the surface. Denoting θ0 the angle between the indenter and the surface, a the contact radius, h the depth of the indentation and s the spacing between slip steps at the surface, the contact angle θ0 can be evaluated by b h = a s. tanθ0 =. (2.2.5). If we assume that the dislocations remain inside a half sphere of volume V = 23 πa3 , it can be shown ([90]) that the density of geometrically dislocations, which is the total length of dislocation loops divided by the volume, becomes ρG =. 3 tan2 θ0 2bh. (2.2.6). √ Using the Taylor relation for the shear stress τ = αµb ρG (statistically stored dislocations are negligible in the indentation problem) and the Tabor’s factor to convert the flow stress into hardness we have σ=. √ 3τ, H = 3σ. (2.2.7). Using the previous relations, the following characteristic form for the depth dependence of the hardness was then derived: H = H0. r 1+. h∗ h. (2.2.8). where H is the hardness for a given depth of indentation, h, H0 , is the hardness in the limit of.

(47) 34 infinite depth and h∗ is a characteristic length that depends on the shape of the indenter, the shear modulus and H0 , see Figure 2.7 for comparison with experimental data from McElhaney et al [78]. Such a model can be used to derive a strain gradient plasticity law. Indeed, a measure of strain gradient in this problem is χ=. tanθ0 a. (2.2.9). in which case the depth dependence of the hardness can be rewritten as. (. σ 2 µ ) ≈ 1 + b( )2 σ0 σ0. (2.2.10). where σ and σ0 represent the flow stress in presence of strain gradient and the flow stress without strain gradient respectively. For power law hardening of the form σ0 = σref n , this can be recast into a new strain gradient plasticity law of the form. (. σ 2 ) = 2n + `χ σ0. (2.2.11). with the strain independent length scale ` given by. ` = b(. µ σref. )2. (2.2.12). The length parameter ` is a function of the Burger’s vector b and other material constants, χ is the effective strain gradient. This model derived by Nix and Gao resembles the phenomenological law of Fleck and Hutchinson, with their length scale interpreted this time in function of material parameters.. 2.2.2. Problem formulation. In this work, we propose a new formulation that takes into account strain gradient effects. The idea will be to postulate an additive decomposition of the energy density into two components: a first component depending on the first deformation gradient (as in section 2.1.1), and a second that is.

(48) l ¼ pha=b. 3 The average GND density can be obtained from rG ¼ l=V , where V ¼ 2=3 pa is the volume of the hemisphere (Nix and Gao, 1998). This gives rG ¼ ð3 tan2 y0 Þ=2bh, which becomes very large at small indentation depth h (as in nano indentation). 35. a. r 0. h. 0. s. Fig. 3. Schematic diagram of geometrically necessary dislocations underneath the indenter (Nix and Gao, 1998) Figure 2.6: Schematic diagram of geometrically necessary dislocations underneath the indenter (Nix and Gao 1998,[90]) W. D. NIX and H. GAO. 416. Depth Dependence of Hardness 10.0 - (111) single crystal Cu. Ho = 0.581 GPa h’ = 1.60 pm. o.ot,““,“““““““““‘,“““,‘l 0. 1. 2. 3 I/h. Fig. 3. Depth dependence. of the hardness. Figure 2.7: Depth dependence. 4. 5. 6. 7. (pm-‘). of (111) single crystal copper, taken from Fig. 1, plotted according to eqn (8). of the hardness of (111) single crystal copper. Source:[90]. a regularization term that entails strain gradients. the mathematical 5.0v,, /, /, In the ‘,_, following, we provide ,. Depth Dependence of ofHardness framework that will be the basis for our formulation strain gradient plasticity within the context cold worked polycrystalline. Cu. of deformation theory.. Ho = 0.834 GPa.